Format  Pages  Price  
28  $60.00  ADD TO CART  
Hardcopy (shipping and handling)  28  $60.00  ADD TO CART  
Standard + Redline PDF Bundle  56  $72.00  ADD TO CART 
Historical Version(s)  view previous versions of standard
Translated Version(s): Russian
More E04.08 Standards Related Products Standard References Find Labs
Significance and Use
4.1 These test methods cover procedures for estimating and rules for expressing the average grain size of all metals consisting entirely, or principally, of a single phase. The grain size of specimens with two phases, or a phase and a constituent, can be measured using a combination of two methods, a measurement of the volume fraction of the phase and an intercept or planimetric count (see Section 17). The test methods may also be used for any structures having appearances similar to those of the metallic structures shown in the comparison charts. The three basic procedures for grain size estimation are:
4.1.1 Comparison Procedure—The comparison procedure does not require counting of either grains, intercepts, or intersections but, as the name suggests, involves comparison of the grain structure to a series of graded images, either in the form of a wall chart, clear plastic overlays, or an eyepiece reticle. There appears to be a general bias in that comparison grain size ratings claim that the grain size is somewhat coarser (^{1}/_{2} to 1 G number lower) than it actually is (see X1.3.5). Repeatability and reproducibility of comparison chart ratings are generally ±1 grain size number.
4.1.2 Planimetric Procedure—The planimetric method involves an actual count of the number of grains within a known area. The number of grains per unit area, N_{A }, is used to determine the ASTM grain size number, G. The precision of the method is a function of the number of grains counted. A precision of ±0.25 grain size units can be attained with a reasonable amount of effort. Results are free of bias and repeatability and reproducibility are less than ±0.5 grain size units. An accurate count does require marking off of the grains as they are counted.
4.1.3 Intercept Procedure—The intercept method involves an actual count of the number of grains intercepted by a test line or the number of grain boundary intersections with a test line, per unit length of test line, used to calculate the mean lineal intercept length, ℓ. ℓ is used to determine the ASTM grain size number, G. The precision of the method is a function of the number of intercepts or intersections counted. A precision of better than ±0.25 grain size units can be attained with a reasonable amount of effort. Results are free of bias; repeatability and reproducibility are less than ±0.5 grain size units. Because an accurate count can be made without need of marking off intercepts or intersections, the intercept method is faster than the planimetric method for the same level of precision.
4.2 For specimens consisting of equiaxed grains, the method of comparing the specimen with a standard chart is most convenient and is sufficiently accurate for most commercial purposes. For higher degrees of accuracy in determining average grain size, the intercept or planimetric procedures may be used. The intercept procedure is particularly useful for structures consisting of elongated grains (see Section 16).
4.3 In case of dispute, the planimetric procedure shall be the referee procedure in all cases.
4.4 No attempt should be made to estimate the average grain size of heavily coldworked material. Partially recrystallized wrought alloys and lightly to moderately coldworked material may be considered as consisting of nonequiaxed grains, if a grain size measurement is necessary.
4.5 Individual grain measurements should not be made based on the standard comparison charts. These charts were constructed to reflect the typical lognormal distribution of grain sizes that result when a plane is passed through a threedimensional array of grains. Because they show a distribution of grain dimensions, ranging from very small to very large, depending on the relationship of the planar section and the threedimensional array of grains, the charts are not applicable to measurement of individual grains.
1. Scope
1.1 These test methods cover the measurement of average grain size and include the comparison procedure, the planimetric (or Jeffries) procedure, and the intercept procedures. These test methods may also be applied to nonmetallic materials with structures having appearances similar to those of the metallic structures shown in the comparison charts. These test methods apply chiefly to single phase grain structures but they can be applied to determine the average size of a particular type of grain structure in a multiphase or multiconstituent specimen.
1.2 These test methods are used to determine the average grain size of specimens with a unimodal distribution of grain areas, diameters, or intercept lengths. These distributions are approximately log normal. These test methods do not cover methods to characterize the nature of these distributions. Characterization of grain size in specimens with duplex grain size distributions is described in Test Methods E1181. Measurement of individual, very coarse grains in a fine grained matrix is described in Test Methods E930.
1.3 These test methods deal only with determination of planar grain size, that is, characterization of the twodimensional grain sections revealed by the sectioning plane. Determination of spatial grain size, that is, measurement of the size of the threedimensional grains in the specimen volume, is beyond the scope of these test methods.
1.4 These test methods describe techniques performed manually using either a standard series of graded chart images for the comparison method or simple templates for the manual counting methods. Utilization of semiautomatic digitizing tablets or automatic image analyzers to measure grain size is described in Test Methods E1382.
1.5 These test methods deal only with the recommended test methods and nothing in them should be construed as defining or establishing limits of acceptability or fitness of purpose of the materials tested.
1.6 The measured values are stated in SI units, which are regarded as standard. Equivalent inchpound values, when listed, are in parentheses and may be approximate.
1.7 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
1.8 The paragraphs appear in the following order:
Section  Number 
Scope  1 
Referenced Documents  2 
Terminology  3 
Significance and Use  4 
Generalities of Application  5 
Sampling  6 
Test Specimens  7 
Calibration  8 
Preparation of Photomicrographs  9 
Comparison Procedure  10 
Planimetric (Jeffries) Procedure  11 
General Intercept Procedures  12 
Heyn Linear Intercept Procedure  13 
Circular Intercept Procedures  14 
Hilliard SingleCircle Procedure  14.2 
Abrams ThreeCircle Procedure  14.3 
Statistical Analysis  15 
Specimens with Nonequiaxed Grain Shapes  16 
Specimens Containing Two or More Phases or Constituents  17 
Report  18 
Precision and Bias  19 
Keywords  20 
Annexes: 

Basis of ASTM Grain Size Numbers  Annex A1 
Equations for Conversions Among Various Grain Size Measurements  Annex A2 
Austenite Grain Size, Ferritic and Austenitic Steels  Annex A3 
Fracture Grain Size Method  Annex A4 
Requirements for Wrought Copper and CopperBase Alloys  Annex A5 
Application to Special Situations  Annex A6 
Appendixes: 

Results of Interlaboratory Grain Size Determinations  Appendix X1 
Referenced Adjuncts  Appendix X2 
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
ASTM Standards
E3 Guide for Preparation of Metallographic Specimens
E7 Terminology Relating to Metallography
E407 Practice for Microetching Metals and Alloys
E562 Test Method for Determining Volume Fraction by Systematic Manual Point Count
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
E883 Guide for ReflectedLight Photomicrography
E930 Test Methods for Estimating the Largest Grain Observed in a Metallographic Section (ALA Grain Size)
E1181 Test Methods for Characterizing Duplex Grain Sizes
E1382 Test Methods for Determining Average Grain Size Using Semiautomatic and Automatic Image Analysis
ICS Code
ICS Number Code 19.120 (Particle size analysis. Sieving)
UNSPSC Code
UNSPSC Code
DOI: 10.1520/E0112
ASTM International is a member of CrossRef.